Presentation on theme: "COPPER-PLATED STAINLESS STEEL FOR BIPOLAR PLATES IN DIRECT-OXIDATION SOFC."— Presentation transcript:
COPPER-PLATED STAINLESS STEEL FOR BIPOLAR PLATES IN DIRECT-OXIDATION SOFC
INTRODUCTION Direct oxidation of dry hydrocarbon in SOFC CeO 2, Cu catalyst in anode 700 o C Gas-tight seals for an SOFC with a Cu- based anode in a stainless-steel bipolar plate Carbon formation is prevented when the steel is electroplated with a thin Cu film. Basic study for large scale stack and multi-stacking
Experiment Double casting and calcined at 1550 o C for; –Porous Anode: 2.5 2.5 cm 2, 600 m 10 wt% Ceria, 20wt% Cu as catalyst Poreformer : PMMA, Graphite –electrolyte: 90 m Cathode: LSM (La 0.8 Sr 0.2 MnO 3 ) + YSZ calcined at 1250 o C –1~3 cm 2 Cell holder: 430 Stainless steel –Fuel channel made by CNC machine sealing: Commercial Ceramic sealing Copper plating on fuel channel –by using copper Sulfate bath –To prevent catalytic carbon deposition formed by Ni, Fe in stainless steel Analysis for carbon deposition –GCMS Series connection of fuel between two cell for high conversion 1 5 4 6 3 1: Stainless steel stack 2: Cu-cermet anode 3: Electrolyte 4: Cathode 5: Pt current collector 6: Ceramic seal 6 2 Schematic diagram of the SOFC mount used in this study.
V-i Curves & AC-Impedance Analysis Cell potential and power density vs. current density while running on H 2 and n-butane at 973 K. The squares are for H 2 and the circles for n-butane. Power density : 0.16 W/cm 2 for H 2, 0.09 W/cm 2 for butane
Long Run Test for Hydrocarbon Cell performance in n-butane as a function of time at 973 K while holding the cell potential at 0.5 V. Very stable performance during 90 hours
Before and After Test Photograph of cell mount before (a) and after (b) exposure to n-butane at 973 K for 24 hrs. Copper plating on Fuel Channel for reducing the catalytic carbon deposition enduced by Ni, Fe in stainless steel Thin carbon deposition on Copper layer after test –Easily removed by toluene and analyzed by GCMS (a)(a) (b)(b)
Analysis for Carbon Deposition Table 1. Names and molecular weights for selected products that are shown in Figure The GC trace obtained from the carbonaceous deposits formed on Cu-plated stainless steel following exposure to n-butane at 973 K for 24 hours. The structures of selected species are given, along with numbers corresponding to the compounds in Table 1. Poly-Aromatic Hydrocarbons (PAHs) with 2~6 benzene rings
Multi-Stage Connection for High Conversion 2-series connection High conversion of fuel OCV –2.1V for H 2 –1.9V for butane Power density –0.29 W/cm 2 for H 2 –0.16 W/cm 2 for butane Cathode Anode Cathode Anode Fuel High conversion H2H2 butane
Conclusion It is possible to obtain gas-tight seals for an SOFC with a Cu-based anode in a stainless-steel bipolar plate The tar-like substances on Cu plating analyzed by GC-MS consist primarily of poly-aromatic hydrocarbons having between 2~6 aromatic rings. These compounds are probably form as a result of gas-phase, free-radical reactions. It is important to note that these deposits are very different from what is formed in the presence of a metal catalyst such as Ni or Fe. The series-fuel providing to multi-stage cells can increase the conversion and efficiency of fuel.